Indian Journal of Fibre & Textile Research Vol. 33, March 2008, pp. 73-79
Effluent treatment in textile wet processing Bleaching of polyester-cotton fabric
A I Wasif, S K Chintaa & H T Deo
Department of Textiles, D.K.T.E.S Textile & Engineering Institute, Ichalkaranji 416 115, India Revised received 9 April 2007; accepted 21 June 2007
Ecofriendly processes have been developed for the bleaching of carbonized and uncarbonized polyester-cotton blended fabrics with a view to reduce the water consumption and processing time. There is no significant difference in the whiteness values, K/S values and fastness properties of samples bleached by the conventional method and those bleached by the two suggested formulations. Further, by employing ecofriendly processes, there is significant decrease in volume of effluent generated. Both the formulations are found to be techno - economically viable.
Keywords: Bleaching, Ecofriendly processing, Effluent treatment, Polyester - cotton blend, Wet processing IPC Code: Int. Cl.8 D06L3/00
1 Introduction Processing units discharge thousand tones of pollutants especially in the form of BOD (biological oxygen demand), COD (chemical oxygen demand) and TDS (total dissolved solids).1 As a result, the running costs relating to the washing medium (water supply and effluent purification) are very high.2 Although managing waste water from the textile industry is very difficult, it can be dealt with successfully by beginning at the source to minimize the waste water that is produced and the amount of the chemicals present. Various waste water treatment processes are available which can be used to treat the waste water from this industry. However, it cannot be assumed that a simple system can be placed at any textile plant to successfully treat the waste water.3-5 Successful waste water treatment of textile effluent requires thorough investigation of waste water characteristics, source reduction and the application of cleaner production principles, such as chemical substitution and process modifications to make the process of the final effluent treatment as simple as possible.6-8 At the moment, bleaching is in the midst of a reorientation triggered by AOX problem and the ecotextile wave. While in many textile sectors, chlorine chemicals can be dispensed with completely, there is still no fully equivalent alternative to the combined hypochlorite and peroxide process for bleaching cotton knitted fabrics to full white.9,10
Lokhande and Wasif11,12 have developed ecofriendly bleaching process both for cotton and polyester- cotton blended fabrics, wherein potassium permanganate was used for bleaching in place of hypochlorite used in conventional bleaching followed by hydrogen peroxide bleaching with advantage. Deo and Chinta have used redox system for bleaching with hydrogen peroxide, wherein without affecting the quality of bleaching the effluent load has been reduced drastically both for cotton fabric13 and yarn.14 Deo and Paul15 have developed an enzymatic method of carbonization by applying cellulase enzymes repeatedly on polyester-cotton fabrics for the complete removal of cotton component. In the present work, an attempt has been made to reduce the effluent load during the carbonization and bleaching of polyester-cotton fabric for the decentralized processing sector. The bleaching of polyester-cotton blends after carbonization generates huge amount of effluent having high acidic pH and has to be treated separately. The cost of conventional effluent treatment is very high and hence an attempt has been made to modify the process so as to reduce the volume of effluent generated, thereby reducing the treatment cost.
2 Materials and Methods
2.1 Materials Polyester-cotton (65:35) blended fabric (grey width, 48inch; ends per inch, 80; picks per inch, 84; warp count, 80 den; and weft count, 80 den) was used
___________ aTo whom all the correspondence should be addressed. E-mail: email@example.com / firstname.lastname@example.org
INDIAN J. FIBRE TEXT. RES., MARCH 2008
for bleaching after carbonization and polyester-cotton (65:35) blended fabric (grey width, 48inch; ends per inch, 40; picks per inch, 40; warp count, 88 den; and weft count, 80 den) was used for bleaching without carbonization. The above blended fabrics have been chosen for the study as these were commonly used for bleaching in decentralized processing sector. Caustic soda, sodium hypochlorite, hydrogen peroxide, sulphuric acid, soda ash, sodium hydrosulphite, diammonium phosphate and acetic acid, all of AR grade, were used. Peroxide stabilizer AWNI, hydrated calcium oxide, alum, polyelectrolyte, and activated carbon, all of commercial grade, were used. Coralene Brill.Red F3BS (Disperse Red 343) and Chemifix Brill. Red HE7B (Reactive Red 141) dyes were used. 2.2 Methods The experiments were carried out first in the laboratory and then scaled up on the industrial scale in decentralized process house. The fabric was bleached by conventional method as well as by using laboratory prepared Formulations I and II. The processing sequence was changed in both the formulations and the effluent generated was collected for the analysis. The results obtained have been compared with those of conventional method of bleaching. Bulk trials for conventional bleaching process as well as the proposed modified Formulation I and Formulation II were carried out in a decentralized typical process house. The batch size of the fabric was 100 kg. The chemicals (commercial grade) used were purchased by the process house in bulk as per the usual practice of the industry. 2.3 Bleaching of Carbonized Blended Fabric 2.3.1 Conventional Bleaching Process The polyester-cotton blended fabric after loading on jigger was run for two ends in 70% sulphuric acid followed by two ends for aeration and two ends for cold wash. The fabric was neutralized by running for two ends in soda solution followed by two cold washes. The fabric was given two ends in sodium hypochlorite solution (3 gpl available chlorine) at room temperature. The fabric was then given aeration by running two ends followed by two more ends for washing. The fabric was then treated with 0.3% hydrogen peroxide (50%), 0.5% soda ash and 0.15% stabilizer AWNI for four ends at 80C. The fabric was
run for two ends for washing and neutralized with dilute acetic acid. 2.3.2 Formulation I The polyester-cotton blended fabric after loading on jigger was carbonized in the above manner and after adjusting the pH at 10, it was run for four ends in 0.4% hydrogen peroxide (50%), 0.5% soda ash and 0.15% stabilizer AWNI at 80C followed by two cold washes and neutralization. 2.3.3 Formulation II The polyester-cotton blended fabric after loading on jigger was carbonized in the above manner and after adjusting the pH at 10, the fabric was run for two ends in 0.25% solution of sodium hydrosulphite at room temperature. Later 0.4% hydrogen peroxide (50%) and 0.5% soda ash were added to the same bath and four ends were given at 80C. The fabric was then washed by running two ends in water and neutralized. 2.4 Bleaching of Uncarbonized Blended Fabric 2.4.1 Conventional Bleaching Process The polyester-cotton blended fabric after spotting and loading on jigger was run for four ends for scouring with 0.3% caustic soda, 0.6% soda ash, 0.1% wetting agent at boil followed by two ends in hot water and two ends in cold water. The fabric was then treated with sodium hypochlorite (2.0 gpl available chlorine) at room temperature for four ends. The fabric was then run for two ends for cold wash. The fabric was given four ends in 0.75% hydrogen peroxide (50%), 0.5% soda ash, 0.25% stabilizer AWNI and 0.5% optical whitener at 80C and run for two ends for washing and two ends through acetic acid for neutralization. 2.4.2 Formulation I The polyester-cotton blended fabric after spotting and loading on jigger was run for four ends for scouring with 0.3% caustic soda, 0.6% soda ash, 0.1% wetting agent at boil. The fabric was given two ends in hot water wash followed by two ends in cold water wash. The fabric was then treated for two ends with 0.25% sodium hydrosulphite and in the same bath 0.75% hydrogen peroxide (50%), 0.5% soda ash, 0.25% stabilizer AWNI and 0.5% optical whitener were added and four ends were given at 80C. The fabric was washed by running two ends in water and two ends through acetic acid for neutralization.
WASIF et al.: BLEACHING OF POLYESTER-COTTON FABRIC
2.4.3 Formulation II The polyester-cotton blended fabric after spotting and loading on jigger was given combined scouring cum bleaching in the same bath. Fabric was given four ends in a solution containing 0.1% wetting agent, 1% caustic soda, 0.5% reducing agent, and 0.25 % stabilizer AWNI. In the same bath, 0.75% hydrogen peroxide (50%) was added in two installments and total six ends were given. In the second installment, along with hydrogen peroxide 0.5 % optical whitening agent (2B) was added. The scoured bleached fabric was given two ends in hot water followed by two ends in cold water and two ends through acetic acid for neutralization. All the fabrics bleached by conventional and Formulations I and II were dried on stenter at 80C. Eleven minutes are required to complete one end on jigger. 2.5 Treatment of Effluent The effluent16,17 from all the unit processes, like desizing, scouring and bleaching, was collected and treated as per the process sequence shown in Fig. 1. 2.6 Testing and Analysis The whiteness of bleached fabrics was measured on a high volume tester (930 Colorimeter). This instrument directly gives the values of reflection and whiteness (Hunter Scale). The pH, suspended solids (SS), tot